Enhancing Prediction Accuracy In Sift Theory


 Aubrey Allen
 2 years ago
 Views:
Transcription
1 18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department of Mechanical & Aerospace Engineering, Monash University, Clayton, Australia * Corresponding author Keywords: SIFT, matrix failure, polymer composite, failure prediction 1 Introduction In the conventional laminate theory widely used to predict the strength of fibrereinforced polymer composites, the laminae are treated as homogeneous orthotropic materials. Gosse and Christensen [1] adopted a micromechanical approach which predicts separately the failure of the polymer matrix and fibres 1. They used strain invariants as failure criteria and thus this approach was named as Strain Invariant Failure Theory (SIFT). In the application of SIFT, a microstructure analysis is conducted on a unit cell of the composite material that contains a fibre and surrounding polymeric matrix to determine the relationship between the stressstrain states of the whole cell and its matrix and fibre components. This relationship is then used in a structural analysis to predict matrix or fibre failure. In a linear finite element method, the SIFT analysis could be implemented during post processing the results from a computation based on the conventional laminate theory, by correlating the element stressstrain state with matrix and fibre stressstrain states. This theory has been used by a number of researchers and some success has been reported []. For the matrix failure prediction, Gosse and Christensen proposed that two properties that control damage in the matrix, are the first invariant of the strain tensor, J1, and the second invariant deviator, : J = { } 0. 5 = 0.5 [( 1 ) + ( 1 ) + ( ) ] () 1,, are principal strains. where 1 In principle this micromechanical approach may also predict the interfacial failure between the fibre and matrix. These two strain variants can indicate matrix initial failure due to volume increase (dilational strain) and distortional strains respectively. When either of these reaches its critical value, failure will occur. Note that Equation is essentially Von Mises equivalent strain. This paper aims to demonstrate the accuracy of matrix failure prediction could be increased significantly by enhancing these two failure criteria. Discussion about Polymer Failure Criteria In the following discussion four basic load cases will be considered, namely uniaxial compression, pure inplane shear, uniaxial and biaxial, refer to Figure 1. In most part of this paper, only the initial matrix failure is considered, that is the discussion is restricted to the linear elastic condition. (The application to prediction of matrix ultimate failure will be briefly discussed in Section.4.) The stress and strain states under the four load cases are: Uniaxial compression 1 <0, = =0; 1 = 1 /E<0, = = λ 1 Pure inplane shear 1 >0, = 1, =0; 1 =(1+λ) 1 /E>0, = 1, =0 Uniaxial 1 >0, = =0; 1 = 1 /E>0, = = λ 1 Biaxial 1 = >0, =0; 1 = =(1λ) 1 /E, = λ 1 where 1, and are principal stresses, E is the Young s modulus and λ is the Poison s ratio Fig.1. Four basic load cases considered.1 Uniaxial Compression and Pure Shear Cases In terms of the SIFT theory, the failure criterion based on Equation applies to these two cases.
2 It is well known that the strength of polymer materials could be affected by compressive hydrostatic stress. For those polymer materials, to cover both uniaxial compression and pure shear load cases, a yield criterion such as the DruckerPrager criterion [] would be more suitable than Von Mises criterion. Table 1 provides yield strength data for two typical resin materials used in laminate composites. Table 1. Typical resin material strength data [4] Resin Tensile () Compression () Shear () Type 1 Yield strength E=.6GPa Ultimate λ=0.5 strength Type Yield Strength E=.9GPa λ=0.5 Ultimate strength For the prediction of yield strength, if we generate the critical value of from pure shear data, the measured yield strength in the uniaxial compression case will be higher than the predicted using Equation by 11% and 60% respectively for these two materials. This discrepancy can be removed by applying the parameter DruckerPrager criterion (based on Equation ). + BJ1 = A () where and J1 are calculated using Equations 1 and with the measured failure data from compression and shear tests (Table 1); A and B are two parameters determined from this equation. Failure is predicted when: ' = + BJ1 = A (4) where ' is the revised equivalent strain. Equations (5) and (6) below describe the first invariant of the stress tensor, J1, and the second stress invariant deviator, : J = + (5) { } 0. 5 = 0.5 [( 1 ) + ( 1 ) + ( ) ] (6) Only basic failure criteria that are relatively easy to implement are considered in this study. Note the following relationship: 1+ λ = (7) E 1 λ J1 = J1 (8) E The failure prediction equations can alternatively be expressed using stress variables with full equivalence. For isotropic materials, a stress based failure criterion is more commonly used since it is often easier to use and have clearer physical meaning (e.g. hydrostatic pressure effect shown in DruckerPrager criterion). Alternative equations of Equations () and (4) expressed in stresses are: BJ1 A (9) + = = + BJ1 = ' A (10) For the materials listed in Table 1, A and B values calculated are listed in Table. Table. Parameter A and B values Resin Strain based equation Stress based equation A B A B Type 1.5x10 µ Type 1.6x10 µ Uniaxial and Biaxial Tension Cases Before discussing the uniaxial and biaxial cases, we may consider an extreme case where the polymer is loaded with uniformly distributed tensile stress in all the three axial directions. It is well known that the Von Mises yield criterion is not valid in this situation. A DruckerPrager criterion established using parameters determined from compression and shear load cases would also significantly overpredict the strength in this situation. One commonly adopted approach is to use a maximum tensile stress or strain criterion to handle such tensile dominated load conditions, in conjunction with other criteria such as Von Mises or DruckerPrager to handle other load conditions. In contrast, Equation 1 adopted by Gosse and Christensen contains all the principal strain components in linear combination that indicates the volume increase of the material. Bardenheier [56] provided experimental data from uniaxial and biaxial tests of three types of polymer materials. Analysing these data, it is indicated that under a biaxial tensile load condition, prediction based on Equation 1 would significantly
3 underestimate the material strength, refer to Table. The dilational failure could be more accurately predicted using the critical value of, for example: 0.5 J 1 ' = ( ) (11) This fits more closely to the experimental results. Note that as principal stresses are used, Equation 11 is unaffected by any transformation of coordinates. Table. Data from neat resin biaxial tests [56] and errors with different prediction methods Resin Stress applied* Error with prediction method** (%) 1 Eqn Eqn (11) Max stress criterion Type A Type B Type C * Expressed using the ratio of the yield stress in the biaxial test against that in the uniaxial tensile test ** In each method, the yield stress from the uniaxial tensile test was used to determine the critical value for prediction of yield strength in biaxial tests. A + sign means overprediction and a  sign means underprediction.. Combined Failure Envelope Figure illustrates a failure envelope with the planestress condition ( 0). The portion of the failure envelope formed with the DruckerPrager failure criterion has two parts. The solid line part ( CS ) is established with the uniaxial compression and pure shear test data as discussed in Section.1, whilst the fine dot line part ( ST ) is established with the pure shear and uniaxial tensile data in a similar way. This figure shows that the portion of the failure envelope formed with the DruckerPrager failure criterion can intersect with uniaxial compression, pure shear and uniaxial tensile test data points and join with the J 1 curve smoothly, that indicates significantly improvement. (Regarding the curve smoothness, note that a significant improvement of the VonMises criterion over the maximum shear (Tresca) criterion is that it smooths the curve and removes the singular points in Tresca criterion.) In the dimensional space with 1,, coordinate axes, the failure envelope is represented by two cone surfaces (formed with the DruckerPrager failure criterion, with the axis along the line 1 = = and joined at = 0) truncated by a hemisphere surface (formed with J 1 = the uniaxial tensile yield stress). UC CS J 1 UT ST J 1UT UT = uniaxial tensile; BT = biaxial tensile; PS = pure shear; UC = uniaxial compression; UC = with critical value determined from uniaxial compression test; CS = with parameters determined from uniaxial compression and shear tests; ST = with parameters determined from shear and uniaxial tensile tests; J 1UT = J 1 with critical value determined from uniaxial tensile test; and J 1 UT = J 1 with critical value determined from uniaxial tensile test. Fig.. Illustration of failure envelope (planestress).4 Matrix Ultimate Failure Prediction By using the ultimate strength and secant stiffness to replace yield strength and initial linear stiffness, the above analysis may be extended to cover prediction of matrix ultimate failure with linear analyses. Note that: The accuracy of DruckerPrager criterion over Von Mises failure criterion has been clearly observed particularly for the ultimate strength of many polymer materials; and Use of a linear analysis with secant stiffness to approximate a nonlinear analysis is a widely used analysis method and thus may be significant for practical applications. Lamina Unit Cell Analysis A unit cell analysis using a finite element method was further conducted with the four typical load cases discussed above. The failure prediction based on Equation and Equation () was compared with that based on Equations (10) and (11) when both fibre and matrix are present. 1
4 As the discussion in Section indicated that the failure criteria proposed in this paper could predict neat resin failure more accurately, Equations (10) and (11) are used as a yardstick in this comparison..1 Finite Element Model The following typical material properties are assumed: Fibre Young s modulus (E f ) = 00 GPa Fibre Poisson ratio (λ f ) = 0. Matrix Young s modulus (E m ) =.6 GPa Matrix Poisson ratio (λ m ) = 0.5 Fibre volume fraction (V f ) = 0.5 Referring to Figure, with a relatively low fibre volume fraction of 0.5, a square pattern fibre distribution in the matrix can be assumed (as opposed to a hexagon pattern). A unit cell was extracted with two different orientations. A FEM model is shown in Figure 4. Considering the symmetrical condition, only one eighth of the unit cell was built. remaining unloaded surfaces were given a uniform displacement, that results in the gross load on the surface being zero, to reflect the Poisson effect. The loading and boundary conditions applied ensure all the surfaces are kept straight, as required for simulation of a unit cell in a lamina structure.. Results and Discussion..1 Compression and Shear Load Cases The unit cell shown in Figure (a) was considered. As expected, for the matrix material in the uniaxial compression case, high compressive stress concentration (over 4 times the average strain of the unit cell) occurred at the area indicated in Figure 5(a). Due to the Poisson effect from the stiff fibre, the other two stress components perpendicular to the applied load are also compressive in the high stress concentration area. This results in a relatively high hydrostatic stress in this area and thus the strength predicted with the DruckerPrager type criterion is much higher than that with VonMises criterion. In contrast, in the pureshear case, high compressive and tensile stress concentration occurred separately at the areas shown in Figure 5(b). This results in strength predicted with DruckerPrager type criterion to be much less than that with VonMises criterion in the tensile stress concentration area. Compression stress concentration area Tensile stress concentration area (a) Orientation 1 (b) Orientation Fig.. Unit cells with two orientations (V f = 0.5) (a) (b) Fig.5. Stress concentration areas in uniaxial compression and pure shear load cases Fig.4. A unit cell FEM mesh (oneeighth model of the unit cell in Figure a) The load condition is applied in the form of uniform surface displacement. Symmetry boundary conditions are applied to three orthogonal surfaces. The With a load applied that resulted in 0.01 gross strain, the calculated maximum effective stress values are listed in Table 4. For practical applications of the SIFT approach, the failure strength of the matrix is generally determined using laminate specimen tests rather than from neat 4
5 resin tests [1]. If the strength is calibrated using the uniaxial compression strength for Material Type 1 (Table 1), when predicting strength in the pureshear load case, as indicated in Table 4, the difference between the original SIFT approach and the proposed revised approach is 60.6%. Table 4. Predicted maximum and values under uniaxial compression and pureshear loadings Uniaxial compression () Pureshear Ratio ()/ Discrepancy E.00E %.. Uniaxial and Biaxial Tension Load Cases Figure 6 shows the stress concentration areas in these two load cases for the unit cell shown in Figure (a). In the biaxial case, each of the two stress concentration areas was affected mainly by one of the two loads. Thus there is no significant biaxial tensile stress. Table 5 lists maximum J 1 and J 1 values. Consequently when using the two different methods calibrated using uniaxial tensile state data to predict biaxial state strength, the difference is only.4%. Tensile stress concentration areas (a) (b) Fig.6. Stress concentration areas in uniaxial and biaxial load cases  Orientation 1. The unit cell shown in Figure (b) was subsequently calculated. The maximum critical value locations in the uniaxial tensile load case are at a positions shown in Figure 7 (a), whilst the maximum critical The effect of scale difference between the unit cell and lamina structure is generally not considered in SIFT, refer to [1], whilst this calibration may, to certain degree, take the scale effect into consideration. value locations in the biaxial tensile load case are at b positions shown in Figure 7(b). These maximum critical values listed in Table 6. Table 5. Predicted maximum J 1 and J 1 values under uniaxial and biaxial loadings  Orientation 1 Uniaxial () Biaxial Ratio ()/ Discrepancy J J 1.7E a b a.1e % a b a (a) (b) Fig.7. Stress concentration areas in uniaxial and biaxial load cases  Orientation. As shown in Table 6, when using the two different methods calibrated using uniaxial tensile state data to predict biaxial state strength, the difference is 6.1%, in terms of the maximum critical values in the whole matrix, however, for a specific critical location such as at b locations, the two methods yield significant difference. This might have a complicated effect on determining the correlation between the element stressstrain and matrix and fibre stressstrain states. Table 6. Predicted J 1 and J 1 values at critical points under uniaxial and biaxial loadings  Orientation Point a Point b Max Uniaxial () Biaxial Ratio ()/ J Difference J E.44E. 1.0 % J J 1 1.0E.05E % J J E.05E % 5
6 4 Summary The SIFT failure theory separably predicts fibre and matrix failure in a fibre reinforced composite material. Matrix yield prediction is based on a VonMises strain and first strain invariant criteria. Improvement of the matrix failure criteria for prediction accuracy is discussed and demonstrated in this paper. For two typical resin materials, VonMises yield criterion is unable to fit both yield strength values from uniaxial compression and pureshear tests. When calibrated using the measured shear yield strength, the discrepancy between the predicted and measured uniaxial compression strength is found to be 11% and 60% respectively, whilst using a DruckerPrager criterion these discrepancies could be removed. Use of the critical value of the first invariant strain, when calibrated using the uniaxial tensile yield strength, underpredicts the biaxial tensile strength significantly by over 0% on average, compared with available measurement data of neat resin materials. A revised criterion proposed in this paper could reduce the discrepancy to less than 10%. The proposed failure envelope contains Drucker Prager failure criteria, that intersect with all the uniaxial compression, pure shear and uniaxial tensile test data points, and a revised tensile failure criterion. The areas governed by these criteria join each other smoothly. For a unit cell with a fibre and surrounding matrix from a lamina with 50% fibre volume fraction and typical material properties, a FEM analysis conducted in this study indicates that the difference between the yield strength of the matrix material predicted using VonMises and Drucker Prager type criteria is over 60% in the pure shear load case, when the critical values of these yield criteria are determined in the uniaxial compression load case. The FEM analysis showed that the difference between the yield strength of the matrix material in a unit cell predicted using the first strain variant and the revised criterion reaches 6.1% in the biaxial tensile load case, when the critical values of these yield criteria are determined in the uniaxial tensile load case. By using ultimate strengths and secant stiffness to replace yield strengths and initial linear stiffness, the analysis in this paper may be extended to prediction of matrix ultimate failure using linear analyses. Acknowledgement The authors would like to acknowledge that this paper is outcome of a research project of the Cooperative Research Centre for Advanced Composite Structures (CRCACS). References [1] Gosse JH, Christensen S., Strain invariant failure criteria for polymers in composite materials, AIA A. Paper AIAA/ASME/ASCE/ASC conference, Seattle, WA, United States, 001. [] Li R, Kelly D, and Ness R. Application of a first invariant strain criterion for matrix failure in composite materials. Journal of composite Materials, 00. 7(): [] Drucker D C and Prager W. Solid mechanics and plastic analysis for limit design. Quarterly of Applied Mathematics, 10 () , 195. [4] Fei Y P. Mechanics of fibre reinforced composite. Tongji University Press. Shanghai [5] Bardenheier. Mechanicaches Versagen von Polymerwerkstooen. HanserVerlag [6] Kolling S, Haufe A, Feucht M, and Du Bois P A. A constitutive formulation for polymers subjected to high strain rates. 9 th International LSDyna Users Conference. Michigan, June 46,
Plasticity R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur
Plasticity R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Joint Initiative of IITs and IISc Funded by MHRD Page 1 of 9 Table of Contents 1. Plasticity:... 3 1.1 Plastic Deformation,
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationModule4. Mechanical Properties of Metals
Module4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stressstrain curves 3) Yielding under multiaxial stress, Yield criteria, Macroscopic
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationLecture #8: Ductile Fracture (Theory & Experiments)
Lecture #8: Ductile Fracture (Theory & Experiments) by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering, Chair of Computational Modeling of Materials in Manufacturing 2015 1 1 1 Ductile
More informationConstitutive models: Incremental plasticity Drücker s postulate
Constitutive models: Incremental plasticity Drücker s postulate if consistency condition associated plastic law, associated plasticity  plastic flow law associated with the limit (loading) surface Prager
More informationAn orthotropic damage model for crash simulation of composites
High Performance Structures and Materials III 511 An orthotropic damage model for crash simulation of composites W. Wang 1, F. H. M. Swartjes 1 & M. D. Gan 1 BU Automotive Centre of Lightweight Structures
More informationSchool of Materials Science and Engineering, UNSW Sydney, Australia 2. School of Mechanical and Manufacturing Engineering, UNSW Sydney, Australia
2 st International Conference on Composite Materials Xi an, 2025 th August 207 PREDICTING THE EFFECT OF TEMPERATURE ON MATRIX CRACKING IN THERMOSET COMPOSITES USING A STRAIN INVARIANT APPROACH Akhila
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationNonlinear FE Analysis of Reinforced Concrete Structures Using a TrescaType Yield Surface
Transaction A: Civil Engineering Vol. 16, No. 6, pp. 512{519 c Sharif University of Technology, December 2009 Research Note Nonlinear FE Analysis of Reinforced Concrete Structures Using a TrescaType Yield
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationSEMM Mechanics PhD Preliminary Exam Spring Consider a twodimensional rigid motion, whose displacement field is given by
SEMM Mechanics PhD Preliminary Exam Spring 2014 1. Consider a twodimensional rigid motion, whose displacement field is given by u(x) = [cos(β)x 1 + sin(β)x 2 X 1 ]e 1 + [ sin(β)x 1 + cos(β)x 2 X 2 ]e
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationExperimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 pebbles
Experimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 s D. Aquaro 1 N. Zaccari ABSTRACT Dipartimento di Ingegneria Meccanica Nucleare e della Produzione University of Pisa (Italy)
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationUse Hooke s Law (as it applies in the uniaxial direction),
0.6 STRSSSTRAIN RLATIONSHIP Use the principle of superposition Use Poisson s ratio, v lateral longitudinal Use Hooke s Law (as it applies in the uniaxial direction), x x v y z, y y vx z, z z vx y Copyright
More informationCONSIDERATIONS CONCERNING YIELD CRITERIA INSENSITIVE TO HYDROSTATIC PRESSURE
CONSIDERATIONS CONCERNING YIELD CRITERIA INSENSITIVE TO HYDROSTATIC PRESSURE ADRIAN SANDOVICI, PAULDORU BARSANESCU Abstract. For distinguishing between pressure insensitive and pressure sensitive criteria,
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationTHE BEHAVIOUR OF REINFORCED CONCRETE AS DEPICTED IN FINITE ELEMENT ANALYSIS.
THE BEHAVIOUR OF REINFORCED CONCRETE AS DEPICTED IN FINITE ELEMENT ANALYSIS. THE CASE OF A TERRACE UNIT. John N Karadelis 1. INTRODUCTION. Aim to replicate the behaviour of reinforced concrete in a multiscale
More informationLecture #6: 3D Rateindependent Plasticity (cont.) Pressuredependent plasticity
Lecture #6: 3D Rateindependent Plasticity (cont.) Pressuredependent plasticity by Borja Erice and Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering, Chair of Computational Modeling
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationA Semianalytical Model for the Simulation of Polymers
A Semianalytical Model for the Simulation of Polymers Paul Du Bois 3, Stefan Kolling 1, Markus Feucht 1 & André Haufe 2 1 DaimlerChrysler AG, Sindelfingen, Germany 2 Dynamore GmbH, Stuttgart, Germany 3
More informationANSYS Mechanical Basic Structural Nonlinearities
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationComposite models 30 and 131: Ply types 0 and 8 calibration
Model calibration Composite BiPhase models 30 and 3 for elastic, damage and failure PAMCRASH material model 30 is for solid and 3 for multilayered shell elements. Within these models different ply types
More informationModelling the behaviour of plastics for design under impact
Modelling the behaviour of plastics for design under impact G. Dean and L. Crocker MPP IAG Meeting 6 October 24 Land Rover door trim Loading stages and selected regions Project MPP7.9 Main tasks Tests
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationA Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials
Dublin, October 2010 A Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials FracMan Technology Group Dr Mark Cottrell Presentation Outline Some Physical
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationConcept Question Comment on the general features of the stressstrain response under this loading condition for both types of materials
Module 5 Material failure Learning Objectives review the basic characteristics of the uniaxial stressstrain curves of ductile and brittle materials understand the need to develop failure criteria for
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationStressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension, compression or shear
Xi an 225 th August 217 Stressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension compression or shear Heyin Qi 1 Mingming Chen 2 Yonghong Duan 3 Daxu
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationMAE 322 Machine Design Lecture 2. Dr. Hodge Jenkins Mercer University
MAE 322 Machine Design Lecture 2 Dr. Hodge Jenkins Mercer University Statics Load Failure Theories to Understand Maximum Normal Stress (MNS) Maximum Shear Stress (MSS) Distortion Energy (DE) CoulombMohr
More informationChapter 6: Plastic Theory
OHP Mechanical Properties of Materials Chapter 6: Plastic Theory Prof. Wenjea J. Tseng 曾文甲 Department of Materials Engineering National Chung Hsing University wenjea@dragon.nchu.edu.tw Reference: W. F.
More informationEQUIVALENT FRACTURE ENERGY CONCEPT FOR DYNAMIC RESPONSE ANALYSIS OF PROTOTYPE RC GIRDERS
EQUIVALENT FRACTURE ENERGY CONCEPT FOR DYNAMIC RESPONSE ANALYSIS OF PROTOTYPE RC GIRDERS Abdul Qadir Bhatti 1, Norimitsu Kishi 2 and Khaliq U Rehman Shad 3 1 Assistant Professor, Dept. of Structural Engineering,
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationClassical fracture and failure hypotheses
: Chapter 2 Classical fracture and failure hypotheses In this chapter, a brief outline on classical fracture and failure hypotheses for materials under static loading will be given. The word classical
More informationCoupling of plasticity and damage in glass fibre reinforced polymer composites
EPJ Web of Conferences 6, 48 1) DOI: 1.151/epjconf/1648 c Owned by the authors, published by EDP Sciences, 1 Coupling of plasticity and damage in glass fibre reinforced polymer composites R. Kvale Joki
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationNumerical Modelling of Blockwork Prisms Tested in Compression Using Finite Element Method with Interface Behaviour
13 th International Brick and Block Masonry Conference Amsterdam, July 47, 2004 Numerical Modelling of Blockwork Prisms Tested in Compression Using Finite Element Method with Interface Behaviour H. R.
More informationMODELING OF CONCRETE MATERIALS AND STRUCTURES. Kaspar Willam
MODELING OF CONCRETE MATERIALS AND STRUCTURES Class Meeting #1: Fundamentals Kaspar Willam University of Colorado at Boulder Notation: Direct and indicial tensor formulations Fundamentals: Stress and Strain
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationBUCKLING COEFFICIENTS FOR SIMPLY SUPPORTED, FLAT, RECTANGULAR SANDWICH PANELS UNDER BIAXIAL COMPRESSION
U. S. FOREST SERVICE RESEARCH PAPER FPL 135 APRIL 1970 BUCKLING COEFFICIENTS FOR SIMPLY SUPPORTED, FLAT, RECTANGULAR SANDWICH PANELS UNDER BIAXIAL COMPRESSION FOREST PRODUCTS LABORATORY, FOREST SERVICE
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationFailure surface according to maximum principal stress theory
Maximum Principal Stress Theory (W. Rankin s Theory 1850) Brittle Material The maximum principal stress criterion: Rankin stated max principal stress theory as follows a material fails by fracturing
More informationMicroplane Model formulation ANSYS, Inc. All rights reserved. 1 ANSYS, Inc. Proprietary
Microplane Model formulation 2010 ANSYS, Inc. All rights reserved. 1 ANSYS, Inc. Proprietary Table of Content Engineering relevance Theory Material model input in ANSYS Difference with current concrete
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationSIMPLIFIED CONCRETE MODELING WITH *MAT_CONCRET_DAMAGE_REL3
SIMPLIFIED CONCRETE MODELING WITH *MAT_CONCRET_DAMAGE_REL3 Leonard E Schwer Schwer Engineering & Consulting Services, Windsor CA, USA and L. Javier Malvar Karagozian & Case Structural Engineers, Burbank
More informationTheory at a Glance (for IES, GATE, PSU)
1. Stress and Strain Theory at a Glance (for IES, GATE, PSU) 1.1 Stress () When a material is subjected to an external force, a resisting force is set up within the component. The internal resistance force
More informationA FAILURE CRITERION FOR POLYMERS AND SOFT BIOLOGICAL MATERIALS
Material Technology A FALURE CRTERON FOR POLYMERS AND SOFT BOLOGCAL MATERALS Authors: William W. Feng John O. Hallquist Livermore Software Technology Corp. 7374 Las Positas Road Livermore, CA 94550 USA
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationInternational Journal of Innovative Research in Science, Engineering and Technology Vol. 2, Issue 7, July 2013
ANALYSIS AND MITIGATION OF STRESS CONCENTRATION FACTOR OF A RECTANGULAR ISOTROPIC AND ORTHOTROPIC PLATE WITH CENTRAL CIRCULAR HOLE SUBJECTED TO INPLANE STATIC LOADING BY DESIGN OPTIMIZATION Shubhrata Nagpal
More informationReference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",
Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationCHAPTER 2 Failure/Fracture Criterion
(11) CHAPTER 2 Failure/Fracture Criterion (12) Failure (Yield) Criteria for Ductile Materials under Plane Stress Designer engineer: 1 Analysis of loading (for simple geometry using what you learn here
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationPredicting Elastic Properties of Unidirectional SU8/ZnO Nanocomposites using COMSOL Multiphysics
Predicting Elastic Properties of Unidirectional SU8/ZnO Nanocomposites using COMSOL Multiphysics Neelam Mishra 1, and Kaushik Das *1 1 School of Minerals Metallurgical and Materials Engineering, Indian
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationNanoindentation of Fibrous Composite Microstructures: Experimentation and Finite Element Investigation. Mark Hardiman
Nanoindentation of Fibrous Composite Microstructures: Experimentation and Finite Element Investigation Mark Hardiman Materials and Surface Science Institute (MSSI), Department of Mechanical and Aeronautical
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationLecture Triaxial Stress and Yield Criteria. When does yielding occurs in multiaxial stress states?
Lecture 5.11 Triaial Stress and Yield Criteria When does ielding occurs in multiaial stress states? Representing stress as a tensor operational stress sstem Compressive stress sstems Triaial stresses:
More informationISHIK UNIVERSITY DEPARTMENT OF MECHATRONICS ENGINEERING
ISHIK UNIVERSITY DEPARTMENT OF MECHATRONICS ENGINEERING QUESTION BANK FOR THE MECHANICS OF MATERIALSI 1. A rod 150 cm long and of diameter 2.0 cm is subjected to an axial pull of 20 kn. If the modulus
More informationA PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL
A PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL P.Palanivelu 1, R.Siva Prasad 2, 1 PG Scholar, Department of Mechanical Engineering, Gojan School of Business and Technology, Redhills, Chennai, India.
More informationLecture #7: Basic Notions of Fracture Mechanics Ductile Fracture
Lecture #7: Basic Notions of Fracture Mechanics Ductile Fracture by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering, Chair of Computational Modeling of Materials in Manufacturing
More informationABSTRACT INTRODUCTION
Optimization of soil anchorages M. Teschner, C. Mattheck Kernforschungszentrum Karlsruhe GmbH, Institut fur Materialforschung II, W7500 Karlsruhe 1, Postfach 3640, Germany ABSTRACT A new optimization
More informationNUMERICAL SIMULATIONS OF CORNERS IN RC FRAMES USING STRUTANDTIE METHOD AND CDP MODEL
Numerical simulations of corners in RC frames using StrutandTie Method and CDP model XIII International Conference on Computational Plasticity. Fundamentals and Applications COMPLAS XIII E. Oñate, D.R.J.
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More information5 ADVANCED FRACTURE MODELS
Essentially, all models are wrong, but some are useful George E.P. Box, (Box and Draper, 1987) 5 ADVANCED FRACTURE MODELS In the previous chapter it was shown that the MOR parameter cannot be relied upon
More informationPractice Final Examination. Please initial the statement below to show that you have read it
EN175: Advanced Mechanics of Solids Practice Final Examination School of Engineering Brown University NAME: General Instructions No collaboration of any kind is permitted on this examination. You may use
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More information1. Background. is usually significantly lower than it is in uniaxial tension
NOTES ON QUANTIFYING MODES OF A SECOND ORDER TENSOR. The mechanical behavior of rocks and rocklike materials (concrete, ceramics, etc.) strongly depends on the loading mode, defined by the values and
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More information2 CONSTITUTIVE MODELS: THEORY AND IMPLEMENTATION
CONSTITUTIVE MODELS: THEORY AND IMPLEMENTATION 21 2 CONSTITUTIVE MODELS: THEORY AND IMPLEMENTATION 2.1 Introduction There are twelve basic constitutive models provided in, arranged into null, elastic
More informationMost of the material in this package is based on a recently published book. This is:
Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Preknowledge It is assumed that the student is familiar with simple concepts of mechanical
More informationA Simple and Accurate Elastoplastic Model Dependent on the Third Invariant and Applied to a Wide Range of Stress Triaxiality
A Simple and Accurate Elastoplastic Model Dependent on the Third Invariant and Applied to a Wide Range of Stress Triaxiality Lucival Malcher Department of Mechanical Engineering Faculty of Tecnology, University
More informationNonlinear Analysis of Reinforced Concrete Shells Subjected to Impact Loads
Transactions of the 7 th International Conference on Structural Mechanics in Reactor Technology (SMiRT 7) Prague, Czech Republic, August 7, 00 Paper # J0 Nonlinear Analysis of Reinforced Concrete Shells
More informationDurability of bonded aircraft structure. AMTAS Fall 2016 meeting October 27 th 2016 Seattle, WA
Durability of bonded aircraft structure AMTAS Fall 216 meeting October 27 th 216 Seattle, WA Durability of Bonded Aircraft Structure Motivation and Key Issues: Adhesive bonding is a key path towards reduced
More informationAmerican Society for Testing and Materials (ASTM) Standards. Mechanical Testing of Composites and their Constituents
Mechanical Testing of Composites and their Constituents American Society for Testing and Materials (ASTM) Standards Tests done to determine intrinsic material properties such as modulus and strength for
More informationEffect of the intermediate principal stress on fault strike and dip  theoretical analysis and experimental verification
Effect of the intermediate principal stress on fault strike and dip  theoretical analysis and experimental verification B. Haimson University of Wisconsin, USA J. Rudnicki Northwestern University, USA
More informationStatic Failure (pg 206)
Static Failure (pg 06) All material followed Hookeʹs law which states that strain is proportional to stress applied, until it exceed the proportional limits. It will reach and exceed the elastic limit
More informationCOMPRESSIVE BEHAVIOR OF IMPACT DAMAGED COMPOSITE LAMINATES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS COMPRESSIVE BEHAVIOR OF IMPACT DAMAGED COMPOSITE LAMINATES Hiroshi Suemasu*, Wataru Sasaki**, Yuuichiro Aoki***, Takashi Ishikawa**** *Department of
More information